Research Article  Open Access
Influence of Nd Substitution by La in on Structural and Transport Properties for Sensing Applications
Abstract
The structural and transport properties of manganites with and 0.2 prepared by solid state reaction route are studied. These compounds are found to be crystallized in orthorhombic structural form. A shift in the metalsemiconductor/insulator transition temperature () towards room temperature (289 K) with the substitution of Nd by La, as the value of is varied in the sequence (0, 0.1, and 0.2), has been provided. The shift in the , from 239 K (for ) to near the room temperature 289 K (for ), is attributed to the fact that the average radius of siteA increases with the percentage of La. The maximum temperature coefficients of resistance (TCR) of ( and 0.2) are found to be higher compared to its parent compound which is almost independent of . The electrical resistivity of the experimental results is explored by various theoretical models below and above . An appropriate enlightenment for the observed behavior is discussed in detail.
1. Introduction
In the past few decades, AMnO_{3}type manganites have been extensively studied because of their richness in physical properties which is due to the simultaneous presence of spin, lattice, and orbital degrees of freedom [1–3]. Significant attention has been paid by many researchers in order to explore their potential for spacious technological applications such as read heads, magnetic information storage, low and highfield magnetic sensors, IR detectors, and numerous other spintronic applications [4–11]. The substituted manganites provide high temperature coefficient of resistance (TCR) in bulk as well as in thin films at room temperature. This will motivate us to explore them for infrared radiation detectors (i.e., IR detector) for night vision applications [12]. Among all perovskite manganites, NdMnO_{3} is an antiferromagnetic insulator, characterized by a superexchange coupling between Mn^{3+} sites. This coupling is facilitated by a single electron predominated by strong correlation effects. On the other hand, partial substitution of Nd^{3+} ions with divalent cations (Sr, Ca, and Ba) results in mixed valance states of Mn, that is, Mn^{3+}/Mn^{4+} which is responsible for the ferromagnetic Zener double exchange mechanism [13].
The most prevalent experimental way of affecting the physical properties of the manganites is either substituting cations at the A or Bsites or varying the oxygen content in the regular perovskite structure [20–22]. The size mismatch at Asite generates internal chemical pressure within the lattice. Due to this structural disorder effect, the local oxygen displacement occurs, ensuing into bond angle fluctuations and bond length variations, further leading to carrier localization in perovskite lattice. This distortion can be controlled by the average size of the Asite cation which in turn modifies the Mn–O–Mn bond angle and Mn–O distances. The Mn–O–Mn bond angle is directly related to the hopping integral between Mn^{3+} and Mn^{4+} degenerate states. Goldschmidt’s tolerance factor is defined aswhere and are the radii of the average Asite and Bsite ions and is the radius of oxygen ion. For, Mn–O–Mn bond angle is decreasing due to rotation of MnO_{6} octahedra which in turn leads to lower symmetric structure. The transport properties of the substituted manganites are influenced by the local distortion of the lattice. This local distortion occurs by the size mismatch of different radii of Asite cation and also by cationic vacancies of rare earth and divalent alkaline earth elements. This disorder is quantified by means of the variance of the Asite cation radius distributiondefined as whereare the fractional occupancies of the species. Thus, the variations in ionic radii at Asites lead to competing phases at a particular temperature, hence influencing electrical and magnetic transport properties of the perovskite manganites.
In the present research, the structural and transport properties of Ndbased manganites with composition (where = 0, 0.1, and 0.2) are studied in order to tune the TCR and for application aspect. The present work is targeted to achieve favorable properties of manganites for IR detector applications.
2. Experimental Details
The polycrystalline samples of , where = 0, 0.1, and 0.2 are synthesized by the solid state reaction route using ingredients Nd_{2}O_{3}, La_{2}O_{3}, SrCO_{3}, and Mn_{2}O_{3}. The mixed powders are calcined at 1100°C in air for 24 hours. Thereafter, powder is pressed into pellets by applying a uniaxial pressure of 45 tons followed by sintering at 1300°C for 5 hours. The sintered pellets are annealed in an oxygen environment at 1000°C for 5 hours to retain the oxygen stoichiometry. The structure and phase purity of the samples are analyzed by powder Xray diffraction (XRD) performed on a diffractometer (PANanalytical X’pert Pro) using CuK_{α} radiation at 40 kV and 30 mA. The resistivity measurement without and with magnetic field (5T) are carried out using a fourprobe method in the temperature range from 5 to 300 K on a quantum design Physical Property Measurement System (PPMS Model no. 6000).
3. Results and Discussion
3.1. XRD Results
The XRD patterns of polycrystalline manganites where (NLSMO 0), 0.1 (NLSMO 1), and 0.2 (NLSMO 2) prepared by solid state route are shown in Figure 1. The XRD patterns of all compounds exhibit singlephase orthorhombic unit cell with Pnma (no. 62, PCPDF ref no. 861534) space group. It can be observed from patterns that the peaks are slightly shifted toward lower angle side with the substitution of Nd by La. This small shift arises due to the mismatch of radius at Asite, that is, larger radius of Laion (1.36 Å) in comparison to the radius of Ndion (1.27 Å) which causes increase in the volume of the lattice. Subsequently, an internal chemical pressure generated within the lattice due to the size mismatch at Asite, which results in slight shift in the peaks of XRD pattern. The increase in tolerance factor from 0.9408 (for NLSMO 0) to 0.9470 (for NLSMO 2) indicates that the Mn–O–Mn bond angle approaches towards angle 180° which reduces the distortion in MnO_{6}. Less distortive structure promotes the hopping integral and reduces the charge localization (especially below 40 K in our case) which is further supported by the resistivity data.
3.2. Electrical Transport
The design and development of uncooled IR detector (Bolometer) require around the room temperature with high TCR for improved sensitivity [12, 23]. The temperaturedependent resistivitiesstudied in the temperature range 5–300 K are shown in Figure 2. All samples are exhibiting metalsemiconductor/insulator transition (). The shift in the , from 239 K (for ) to near the room temperature 289 K (for ), is attributed to the fact that the average radius of siteA increases with the percentage of La. In perovskite manganites, the oxygen ions tend to move towards the center of MnO_{6} octahedra as decreases, which in turn leads to distortion. Hence, average Asite ionic radii induced distortion is influencing the reduction in Mn–O bond distances and Mn–O–Mn bond angle. This lattice distortion offers a localized state for the electron and causes possible electronic phase separation within the lattice. Therefore, hopping amplitude of the charge carrier from Mn^{3+} to Mn^{4+} is decreasing due to suppression of delocalized hopping sites [24]. As the average radius increases, the local lattice distortion reduces due to the shifting of Mn–O–Mn bond angle towards symmetrical side (180°). As a consequence, hopping amplitude increases which leads to shift in towards higher temperature.
In order to understand the electrical transport mechanism of manganites, the temperaturedependent resistivity is categorized into two parts: low temperature and high temperature () behaviors. In case of, TCR is positive (i.e., ), while it is negative () for.
3.2.1. Low Temperature Behavior
Based on the temperaturedependent polynomial equations, the variation of resistivity at low temperatures and comparative strengths of the different scattering mechanisms are explained [14–19]. These equations are used to explain the low temperature resistivity of manganites which is given in Table 1. From these equations, the conduction phenomenon of different scattering mechanisms is well explained.

In the equations, is the temperatureindependent residual resistivity which arises due to the grain/domain boundary effects, scattering by impurities, defects, and domain walls [18, 25]. Since polycrystalline materials have many grain boundaries, their substantial contribution to the resistivity is proved in microwave measurement [26]. Hence, plays a main role in the conduction phenomena. The term describes the resistivity due to electronelectron scattering phenomenon [27, 28], while the term gives resistivity due to the phenomenon of single magnon scattering process in ferromagnetic phase [18, 26, 29]. The last terms ascribe due to the process of electronmagnon scattering process in the ferromagnetic region [28] and contributes to the resistivity due to the phenomenon of electronphonon interaction [19].
The experimental data of our samples are fitted with general polynomial equation and their related fitting graphs and parameters are shown in Figure 3 and Table 2, respectively. From these data, the corresponding fitted parameters are decreasing with increase of Asite average radius . It can be observed from the graphs of Figure 3; the residual resistivity of the original data is slightly higher than the fitting parameter values. This slight variation in residual resistivity arises may be due to the presence of grain boundary effects in the polycrystalline materials as well as localization effects particularly at low temperature. From Figure 4, it can be concluded that the residual resistivity is decreasing with increase of the average radius of Asite. These results are consistent with the reported literature [30]. As shown in Table 2, the values of and are obtained from fitting polynomial (Figure 3) and are also decreasing with increase of Asite average radius .

(a)
(b)
(c)
The observed maximum %TCR versus average radius of Asite, is given in the inset of Figure 4. The maximum %TCR values of the compounds are increasing with average radius of Asite but %TCR values are slightly equal in = 0.1 and 0.2 as compared to the parent compound. It is worth to mention here that %TCR have values 2.66 (for ) and 2.65 (for ) which are independent with. To design a room temperature uncooled resistive bolometer (IR detector), the potential materials are αSi, polycrystalline SiGe, semiconducting YBCO, VO_{2}, and VO_{x} having maximum TCR values of 2% to 6% [31, 32], 7% [33], 2.9% [34], 1.7% [35, 36], and 3.3% K^{−1}) [37], respectively. The present results of our %TCR values are comparative with the existing materials. Hence, the present study enriches the possibility of further improvement in operating around room temperature for bolometer applications without sacrificing an optimum %TCR value.
3.2.2. High Temperature Behavior
In paramagnetic or semiconducting/insulating phase, the electrical resistivity generally exhibits strong temperature dependence. Several conduction mechanisms are used to explain the electrical transport properties at high temperature above . The most prevalent models are used to describe the conduction mechanisms by Mott’s variable range hopping model () [38] and another one small polaron hopping model () where is the Debye temperature [39]. Two models are linearly best fitted with experimental results. The experimental data of NLSMO 2 are fitted within a narrow temperature regime due to higher ; however, the obtained theoretical parameters are reasonably accountable as summarized in Table 3.

According to Mott’s variable range hopping model (VRH), the characteristic hopping length increases with lowering temperature and density of states are obtained from the wellestablished Mott law. Hopping conduction results from the states whose energies are focused in a narrow band near the vicinity of Fermi level is given by the equation where, Boltzmann’s constant, and is the density of states at the Fermi level. Here we have taken value 2.22 nm^{−1} which is estimated and reported for manganites in [40]. values are measured by slope of versus which is useful for measurement of density of the states at the Fermi level, and the values obtained from Figure 5 are given in Table 3. The density of states are increasing with increase of Asite average radius that affect the conducting nature of the samples.
(a)
(b)
(c)
Small polaron hopping models are used to explain the conductivity mechanism by either adiabatic polaron hopping or nonadiabatic polaron hopping. Here is the residual resistivity and is the polaron activation energy. Jung [41] have pointed out that the higher value of is due to the effect of adiabatic small polaron hopping process. The higher order density of states is indicating the applicability of the adiabatic hopping mechanism. Based on this, the adiabatic small polaron hopping model is used in the present investigation rather than nonadiabatic small polaron hopping model. Polaron activation energy of the samples has been obtained from the slopes of versus curves of Figure 6. These values are given in Table 3. Henceforth, it can be concluded that the decrease in polaron activation energies with the increase in average radius occur due to the shift in Mn–O–Mn bond angle towards 180° which is shown in Figure 7. The hopping of charge carrier from one site to another site in the lattice will be enhanced with the decrease of polaron activation energy.
(a)
(b)
(c)
From Table 3, density of statesvalues are increasing with average radius. Thisspecifies the carrier effective mass in other sense narrowing of the band width, consequently results in a large change in the resistivity and sharpening of the resistivity peak in the vicinity of [42]. The higher values of density of states at the Fermi level lead to a higher value of conductivity [41].
3.3. Magnetoresistance
Figure 8 shows the electrical resistivity behavior of the where =0, 0.1, and 0.2 samples in a constant magnetic field of 5T. In the presence of an external magnetic field, the resistivity decreases significantly. This suggests that the external magnetic field (5T) facilitates the hopping of electron between neighbouring Mn ions, which agrees with the double exchange mechanism [13].
(a)
(b)
(c)
The magnetoresistance MR is defined as %MR whereand are the resistivities at temperature without magnetic field and in the applied magnetic field , respectively. The highest percentage MR (at ) values of the are 46%, 52%, and 50% for = 0, 0.1, and 0.2 as shown in inset of Figure 8. The %MR values are increasing slightly higher than the parent compound with varying of ; this will be useful for potential applications [8, 43]. The misalignment of adjacent magnetic domains/grains or phase separation scenario are responsible for lowtemperature MR. Hopping of charge carriers become easier across the domain wall boundaries and the resistivity decreases, which in turn leads to significant MR at low temperature. Colossal magnetoresistance at is due to the alignment of adjacent Mn ions in the presence of field which directly influence the double exchange mechanism.
4. Conclusion
In this paper, the influence of La substitution at Nd site on the electrical and magnetotransport properties in ( = 0, 0.1 and 0.2) has been extensively studied. is shifting towards room temperature with La content. Conduction mechanism behavior is explained by the polynomial equation in lowtemperature region and the hightemperature behavior is described using different prevalent existing models. From the present study, it can be concluded that the residual resistivityand the polaron activation energies are decreasing with increase of average radius of siteA. An interesting observation is that NLSMO 2 provides around the room temperature and maximum percentage of TCR values are independent with average radius in and . However, the TCR value is not satisfactorily high for the development of sensitive microbolometer; this study will be useful in future to optimize the working temperature without affecting the TCR. Moreover, the present research can further be extended for the optimization of the composition to achieve high TCR with around the room temperature for the development of MEMSbased uncooled microbolometer for night vision cameras.
References
 J. M. D. Coey, M. Viret, and S. Von Molnár, “Mixedvalence manganites,” Advances in Physics, vol. 48, no. 2, pp. 167–293, 1999. View at: Google Scholar
 D. H. Manh, P. T. Phong, T. D. Thanh, L. V. Hong, and N. X. Phuc, “La_{0.7}Ca_{0.3}MnO_{3} perovskite synthesized by reactive milling method: the effect of particle size on the magnetic and electrical properties,” Journal of Alloys and Compounds, vol. 491, no. 12, pp. 8–12, 2010. View at: Publisher Site  Google Scholar
 P. K. Siwach, H. K. Singh, and O. N. Srivastava, “Low field magnetotransport in manganites,” Journal of Physics Condensed Matter, vol. 20, no. 27, Article ID 273201, 2008. View at: Publisher Site  Google Scholar
 M. M. Seikh, L. Sudheendra, and C. N. R. Rao, “Magnetic properties of La_{0.5x}Ln_{x}Sr_{0.5}MnO_{3} (Ln = Pr, Nd, Gd and Y),” Journal of Solid State Chemistry, vol. 177, no. 10, pp. 3633–3639, 2004. View at: Publisher Site  Google Scholar
 R. Von Helmolt, J. Wecker, B. Holzapfel, L. Schultz, and K. Samwer, “Giant negative magnetoresistance in perovskitelike La_{2/3}Ba_{1/3}MnO_{x} ferromagnetic films,” Physical Review Letters, vol. 71, no. 14, pp. 2331–2333, 1993. View at: Publisher Site  Google Scholar
 S. Jin, T. H. Tiefel, M. McCormack, R. A. Fastnacht, R. Ramesh, and L. H. Chen, “Thousandfold change in resistivity in magnetoresistive LaCaMnO films,” Science, vol. 264, no. 5157, pp. 413–415, 1994. View at: Google Scholar
 A.M. HaghiriGosnet and J.P. Renard, “CMR manganites: physics, thin films and devices,” Journal of Physics D, vol. 36, no. 8, pp. R127–R150, 2003. View at: Publisher Site  Google Scholar
 J. Heremans, “Solid state magnetic field sensors and applications,” Journal of Physics D, vol. 26, no. 8, pp. 1149–1168, 1993. View at: Publisher Site  Google Scholar
 S. Jin, M. McCormack, T. H. Tiefel, and R. Ramesh, “Colossal magnetoresistance in LaCaMnO ferromagnetic thin films (invited),” Journal of Applied Physics, vol. 76, no. 10, pp. 6929–6933, 1994. View at: Publisher Site  Google Scholar
 J. Mira, J. Rivas, L. E. Hueso, F. Rivadulla, M. A. López Quintela, and C. A. Ramos, “Strong reduction of lattice effects in mixedvalence manganites related to crystal symmetry,” Physical Review B, vol. 65, no. 2, Article ID 024418, 5 pages, 2002. View at: Publisher Site  Google Scholar
 L. Hueso and N. Mathur, “Dreams of a hollow future,” Nature, vol. 427, no. 6972, pp. 301–304, 2004. View at: Publisher Site  Google Scholar
 J.H. Kim and A. M. Grishin, “Freestanding epitaxial La_{1x}(Sr,Ca)_{x}MnO_{3} membrane on Si for uncooled infrared microbolometer,” Applied Physics Letters, vol. 87, no. 3, Article ID 033502, 3 pages, 2005. View at: Publisher Site  Google Scholar
 C. Zener, “Interaction between the dshells in the transition metals. II. Ferromagnetic compounds of manganese with Perovskite structure,” Physical Review, vol. 82, no. 3, pp. 403–405, 1951. View at: Publisher Site  Google Scholar
 P. Schiffer, A. P. Ramirez, W. Bao, and S. W. Cheong, “Low temperature magnetoresistance and the magnetic phase diagram of La_{1x}Ca_{x}MnO_{3},” Physical Review Letters, vol. 75, no. 18, pp. 3336–3339, 1995. View at: Publisher Site  Google Scholar
 E. S. Vlakhov, R. A. Chakalov, R. I. Chakalova et al., “Influence of the substrate on growth and magnetoresistance of La_{0.7}Ca_{0.3}MnO_{z} thin films deposited by magnetron sputtering,” Journal of Applied Physics, vol. 83, no. 4, pp. 2152–2157, 1998. View at: Google Scholar
 A. Urushibara, Y. Moritomo, T. Arima, A. Asamitsu, G. Kido, and Y. Tokura, “Insulatormetal transition and giant magnetoresistance in La_{1x}Sr_{x}MnO_{3},” Physical Review B, vol. 51, no. 20, pp. 14103–14109, 1995. View at: Publisher Site  Google Scholar
 K. Kubo and N. Ohata, “A quantum theory of double exchange. I,” Journal of the Physical Society of Japan, vol. 33, no. 1, pp. 21–31, 1972. View at: Google Scholar
 G. J. Snyder, R. Hiskes, S. DiCarolis, M. R. Beasley, and T. H. Geballe, “Intrinsic electrical transport and magnetic properties of La_{0.67}Ca_{0.33}MnO_{3} and La_{0.67}Sr_{0.33}MnO_{3} MOCVD thin films and bulk material,” Physical Review B, vol. 53, no. 21, pp. 14434–14444, 1996. View at: Google Scholar
 M. Jaime, P. Lin, M. B. Salamon, and P. D. Han, “Lowtemperature electrical transport and double exchange in La_{0.67}(Pb,Ca)_{0.33}MnO_{3},” Physical Review B, vol. 58, no. 10, pp. R5901–R5904, 1998. View at: Google Scholar
 L. Sudheendra and C. N. R. Rao, “Electronic phase separation in the rareearth manganates (La_{1x}Ln_{x})_{0.7}Ca_{0.3}MnO_{3} (Ln = Nd, Gd and Y),” Journal of Physics Condensed Matter, vol. 15, no. 19, pp. 3029–3040, 2003. View at: Publisher Site  Google Scholar
 S. Asthana, D. Bahadur, A. K. Nigam, and S. K. Malik, “Magnetotransport studies on (Pr_{1/3}Sm_{2/3})_{2/3}A_{1/3}MnO_{3} (A = Ca, Sr and Ba) compounds,” Journal of Physics Condensed Matter, vol. 16, no. 29, pp. 5297–5307, 2004. View at: Publisher Site  Google Scholar
 S. Asthana, D. Bahadur, A. K. Nigam, and S. K. Malik, “Lattice effect on the magnetic and magnetotransport properties of (La_{1/3}Sm_{2/3})_{0.67}Ba_{0.33x} Sr_{x}MnO_{3} ($x=0.0$, 0.1, 0.2 and 0.33) compounds,” Journal of Alloys and Compounds, vol. 450, no. 12, pp. 136–141, 2008. View at: Publisher Site  Google Scholar
 G. J. Yong, R. M. Kolagani, S. Adhikari et al., “Heteroepitaxy of Nd_{0.67}Sr_{0.33}MnO_{3} on silicon for bolometric xray detector application,” Review of Scientific Instruments, vol. 81, no. 11, Article ID 113906, 6 pages, 2010. View at: Publisher Site  Google Scholar
 S. Bhattacharya, R. K. Mukherjee, B. K. Chaudhuri, and H. D. Yang, “Effect of Li doping on the magnetotransport properties of La_{0.7}Ca_{0.3y}Li_{y}MnO_{3} system: decrease of metalinsulator transition temperature,” Applied Physics Letters, vol. 82, no. 23, pp. 4101–4103, 2003. View at: Publisher Site  Google Scholar
 J. M. De Teresa, M. R. Ibarra, J. Blasco et al., “Spontaneous behavior and magnetic field and pressure effects on La_{2/3}Ca_{1/3}MnO_{3} perovskite,” Physical Review B, vol. 54, no. 2, pp. 1187–1193, 1996. View at: Google Scholar
 M. Dominguez, S. M. Bhagat, S. E. Lofland et al., “Giant magnetoresistance at microwave frequencies,” Europhysics Letters, vol. 32, no. 4, article 349, 1995. View at: Publisher Site  Google Scholar
 A. Banerjee, S. Pal, and B. K. Chaudhuri, “Nature of smallpolaron hopping conduction and the effect of Cr doping on the transport properties of rareearth manganite La_{0.5}Pb_{0.5}Mn_{1x}Cr_{x}O_{3},” Journal of Chemical Physics, vol. 115, no. 3, pp. 1550–1558, 2001. View at: Publisher Site  Google Scholar
 A. Urushibara, Y. Moritomo, T. Arima, A. Asamitsu, G. Kido, and Y. Tokura, “Insulatormetal transition and giant magnetoresistance in La_{1x}Sr_{x}MnO_{3},” Physical Review B, vol. 51, no. 20, pp. 14103–14109, 1995. View at: Publisher Site  Google Scholar
 L. Pi, L. Zheng, and Y. Zhang, “Transport mechanism in polycrystalline La_{0.825}Sr_{0.175}Mn_{1x}Cu_{x}O_{3},” Physical Review B, vol. 61, no. 13, pp. 8917–8921, 2000. View at: Google Scholar
 S. Asthana, D. Joonghoe, and D. Bahadur, “Effects of Asite ionic size variation on the magnetic and transport properties of (Pr_{x}Sm_{1x})_{2/3}Sr_{1/3}MnO_{3} ($0\le \times \le 1$),” Physica Status Solidi (B), vol. 244, no. 12, pp. 4542–4545, 2007. View at: Publisher Site  Google Scholar
 V. Y. Zerov and V. G. Malyarov, “Heatsensitive materials for uncooled microbolometer arrays,” Journal of Optical Technology, vol. 68, no. 12, pp. 939–948, 2001. View at: Google Scholar
 V. G. Malyarov, “Uncooled thermal IR arrays,” Journal of Optical Technology, vol. 69, no. 10, pp. 750–760, 2002. View at: Google Scholar
 S. Sedky, P. Fiorini, K. Baert, L. Hermans, and R. Mertens, “Characterization and optimization of infrared poly SiGe bolometers,” IEEE Transactions on Electron Devices, vol. 46, no. 4, pp. 675–682, 1999. View at: Publisher Site  Google Scholar
 M. Almasri, Z. ÇelikButler, D. P. Butler, A. Yaradanakul, and A. Yildiz, “Uncooled multimirror broadband infrared microbolometers,” Journal of Microelectromechanical Systems, vol. 11, no. 5, pp. 528–535, 2002. View at: Publisher Site  Google Scholar
 A. P. Gruzdeva, V. Y. Zerov, O. P. Konovalova et al., “Bolometric and noise properties of elements for uncooled IR arrays based on vanadium dioxide films,” Journal of Optical Technology, vol. 64, no. 12, pp. 1110–1113, 1997. View at: Google Scholar
 C. Chen, X. Yi, J. Zhang, and X. Zhao, “Linear uncooled microbolometer array based on VO_{x} thin films,” Infrared Physics and Technology, vol. 42, no. 2, pp. 87–90, 2001. View at: Publisher Site  Google Scholar
 V. Y. Zerov, V. G. Malyarov, I. A. Khrebtov, Y. V. Kulikov, I. I. Shaganov, and A. D. Smirnov, “Uncooled membranetype linear microbolometer array based on a VO_{x} film,” Journal of Optical Technology, vol. 68, no. 6, pp. 428–431, 2001. View at: Google Scholar
 G. F. Dionne, “Magnetic exchange and charge transfer in mixedvalence manganites and cuprates,” Journal of Applied Physics, vol. 79, no. 8, pp. 5172–5174, 1996. View at: Google Scholar
 N. F. Mott, “Conduction in glasses containing transition metal ions,” Journal of NonCrystalline Solids, vol. 1, no. 1, pp. 1–17, 1968. View at: Google Scholar
 M. Viret, L. Ranno, and J. M. D. Coey, “Magnetic localization in mixedvalence manganites,” Physical Review B, vol. 55, no. 13, pp. 8067–8070, 1997. View at: Google Scholar
 W.H. Jung, “Evaluation of Mott's parameters for hopping conduction in La_{0.67}Ca_{0.33}MnO_{3} above T_{c},” Journal of Materials Science Letters, vol. 17, no. 15, pp. 1317–1319, 1998. View at: Google Scholar
 L. S. Ewe, I. Hamadneh, H. Salama, N. A. Hamid, S. A. Halim, and R. AbdShukor, “Magnetotransport properties of La_{0.67}Ca_{0.33}MnO_{3} with different grain sizes,” Applied Physics A, vol. 95, no. 2, pp. 457–463, 2009. View at: Publisher Site  Google Scholar
 W. Zhang, I. W. Boyd, M. Elliott, and W. HerrendenHarkerand, “Transport properties and giant magnetoresistance behavior in LaNdSrMnO films,” Applied Physics Letters, vol. 69, no. 8, pp. 1154–1156, 1996. View at: Google Scholar
Copyright
Copyright © 2013 Sudarshan Vadnala et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.